University of Groningen
Synthesis and evaluation of novel linear and branched polyacrylamides for enhanced oil
Wever, Diego-Armando Zacarias
IMPORTANT NOTE: You are advised to consult the publisher's version (publisher's PDF) if you wish to cite from
it. Please check the document version below.
Publisher's PDF, also known as Version of record
Link to publication in University of Groningen/UMCG research database
Citation for published version (APA):
Wever, D-A. Z. (2013). Synthesis and evaluation of novel linear and branched polyacrylamides for
enhanced oil recovery. Groningen: s.n.
Other than for strictly personal use, it is not permitted to download or to forward/distribute the text or part of it without the consent of the
author(s) and/or copyright holder(s), unless the work is under an open content license (like Creative Commons).
If you believe that this document breaches copyright please contact us providing details, and we will remove access to the work immediately
and investigate your claim.
Downloaded from the University of Groningen/UMCG research database (Pure): http://www.rug.nl/research/portal. For technical reasons the
number of authors shown on this cover page is limited to 10 maximum.
Download date: 11-10-2020
Towards new polymers for enhanced
The progress booked in this project is discussed in terms of the problems
that have been overcome. Control of the acrylamide (AM) polymerization was
accomplished and this allows the preparation of polyacrylamide (PAM) with
variations in its chemical structure and molecular architecture. Branching in
PAM is presented as a new tool to significantly improve the solution viscosity
without changing the chemical structure of the polymer.
The non-ionic nature of the branched PAM renders it insensitive to the
presence of salt. More specifically, the solution viscosity and the elastic
response are not affected by the presence of salt. The rheological properties
of aqueous solutions are maintained when increasing the amount of salt
whereas those of the commercial HPAM are dependent on the salt
The AM units in HPAM are also highly susceptible to alkaline hydrolysis at
high temperatures (T > 50 °C). N,N-dimethyl acrylamide (DMA), as a
hydrolysis resistant moiety, is a viable option especially in combination with
the increase thickening efficiency through branching. The oil recovery
efficiency of the branched PDMA polymers is similar to branched PAMs, as
evaluated using a 2D flow-cell that simulates residual oil trapped in dead-
ends. This makes them interesting polymers for application in EOR where
alkaline agents are used to in situ generate surfactants.
The obtained results constitute a breakthrough in the general field of
chemical product design for EOR. However, a further refinement of the used
criteria can be envisaged on the basis of the changing legislation (e.g.
currently in Norway). This implies the use of biologically degradable polymers
for underground injection as fitting a general “sustainability” concept for this
application. In this context, the potential of different biopolymers for EOR
where synthetic polymers cannot be used is briefly discussed. All the
currently investigated biopolymers are based on polysaccharides, albeit with
slightly different molecular structures. The thickening capability and
Outlook on the application of branched (co)polymers in EOR
resistance towards salt and temperature of the biopolymers are a strong
function of the molecular weight and their ability to form helical structures in
aqueous solutions. The elasticity of the biopolymer solutions are a strong
function of the molecular weight of the biopolymer, with the higher molecular
weight ones displaying a more pronounced elastic response.
Water soluble polymers in EOR have been investigated and applied in
different techniques, i.e. Polymer Flooding, Alkaline Surfactant Polymer (ASP)
Flooding, and Surfactant Polymer (SP) Flooding.1 When water soluble
polymers are applied in any of the former techniques, several different
aspects have to be considered. In the context of this dissertation, i.e. EOR,
the important ones (amongst others) are: the solution viscosity as a function
of the polymer concentration, the dependency of the solution viscosity on the
presence of salt (mono- and divalent ions), and the resistance (in terms of
solution viscosity) towards higher temperatures (T > 50 °C).
The dependency of the solution viscosity on the polymer concentration is
in general well known for homopolymers. The rheological properties depend
on the concentration regime in which the solution is. In general four different
concentration regimes can be distinguished (Figure 8.1).
Figure 8.1: Concentration regimes in polymeric solutions
At low polymer concentration, the polymer coils do not overlap and the
solution rheology can be described2 using Einstein’s equation3 for dilute
solutions of spherical particles:
where = viscosity of the solution, = viscosity of the solvent and = the
volume fraction of the particles.
At these low concentrations, the solution viscosity depends solely on the
volume fraction of the spheres, i.e. the polymer coils, and not on their size.
The polymer concentration at which the polymer coils start to touch (overlap)
each other is defined as the first critical overlap concentration (C*).
According to several estimations, the values for C* generally range between
Outlook on the application of branched (co)polymers in EOR
0.1 up to 5.0 wt.%.3 When the polymer concentration is increased beyond
C*, overlapping of the polymer coils becomes more prominent and the
solution viscosity increases significantly. The concentration regime starting
from the C* up to a second critical concentration (C**, above which a gel is
formed) is defined as the semi-dilute regime. The viscosity of a polymeric
solution in this regime is governed by the relaxation, i.e. reptation4, of the
entanglements in response to disturbances caused by deformation forces
(stresses). At higher concentrations (c > C**, polymer concentration [p] ≥
50 wt.%3), the rheological properties resemble those observed for polymers
in the melt state.3, 5, 6 However, when making allowances for the desired
application (i.e. EOR), the increase in the polymer concentration can lead to
significant problems in the reservoir. The propagation of polymer coils
through narrow pore throats “presses” the coils closer to each other. If the
coils are large enough, bridging (Figure 8.2) can arise which leads to
blockage of pores.7-10
Figure 8.2: Bridging in porous media10
An increase in the polymer concentration is also detrimental for the
economics of a flooding project given the scale of such projects (e.g. for the
Marmul field pilot-project ~25 ton/day of dry polymer has been used11, 12).
The molecular weight also affects the rheological properties of water
soluble polymers. In general, the solution viscosity increases with the
molecular weight of the polymer, and the dependency can be described using
the reptation model of de Gennes.4 At equal polymer concentration, an
increase in the molecular weight will lead to an increase in the overlap
density, which in turn leads to longer relaxation times (synonymous of higher
viscosities). Nevertheless, the molecular weight of the polymers cannot be
increased indefinitely without leading to problems. Sensitivity towards
mechanical degradation becomes a significant problem as the molecular
weight of the polymers increases.13-17 In addition, the aforementioned
problem with bridging will be augmented with an increase in the molecular
weight.8, 9 In practice, high molecular weight HPAM leads to filter cake
formation on the surface (face plugging) of cores, especially low permeable
ones, and cannot be applied in a reservoir field with similar rock properties.18
The introduction of charges (in PAM, the hydrolysis degree) in a polymer
backbone will lead to an increase in the solution viscosity compared to its